#------------------------------------------------------------------------------
#$Date: 2016-03-05 11:53:18 +0200 (Sat, 05 Mar 2016) $
#$Revision: 177818 $
#$URL: svn://www.crystallography.net/cod/cif/7/03/76/7037673.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7037673
loop_
_publ_author_name
'Hu, Yang-Yang'
'Zhang, Ting-Ting'
'Zhang, Xiao'
'Zhao, De-Chuan'
'Cui, Xiao-Bing'
'Huo, Qi-Sheng'
'Xu, Ji-Qing'
_publ_section_title
;
 New organic-inorganic hybrid compounds constructed from polyoxometalates
 and transition metal mixed-organic-ligand complexes.
;
_journal_issue                   6
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              2562
_journal_page_last               2573
_journal_paper_doi               10.1039/c5dt04413h
_journal_volume                  45
_journal_year                    2016
_chemical_formula_sum            'C52 H40 Cl2 Cu4 Ge N10 O46 W12'
_chemical_formula_weight         4144.79
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2015-12-07 deposited with the CCDC.
2015-12-15 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 128.069(3)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   15.1378(9)
_cell_length_b                   13.5053(8)
_cell_length_c                   23.9776(11)
_cell_measurement_reflns_used    8933
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.2080
_cell_measurement_theta_min      3.2330
_cell_volume                     3859.2(4)
_computing_cell_refinement       'CrysAlisPro 1.171.38.41 (Rigaku OD, 2015)'
_computing_data_collection       'CrysAlisPro 1.171.38.41 (Rigaku OD, 2015)'
_computing_data_reduction        'CrysAlisPro 1.171.38.41 (Rigaku OD, 2015)'
_computing_molecular_graphics    'Diamond 3.2'
_computing_publication_material  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'SuperNova, Dual, Cu at zero, Eos'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0440
_diffrn_reflns_av_unetI/netI     0.0506
_diffrn_reflns_laue_measured_fraction_full 0.999
_diffrn_reflns_laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       28
_diffrn_reflns_limit_l_min       -28
_diffrn_reflns_number            19015
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         25.349
_diffrn_reflns_theta_min         2.939
_exptl_absorpt_coefficient_mu    19.433
_exptl_absorpt_correction_T_max  0.098
_exptl_absorpt_correction_T_min  0.043
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.38.41 (Rigaku Oxford Diffraction, 2015)
Analytical numeric absorption correction using a multifaceted crystal
            model based on expressions derived by R.C. Clark & J.S. Reid.
(Clark, R. C. & Reid, J. S. (1995). Acta Cryst. A51, 887-897)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            blue
_exptl_crystal_density_diffrn    3.567
_exptl_crystal_description       block
_exptl_crystal_F_000             3720
_exptl_crystal_size_max          0.340
_exptl_crystal_size_mid          0.250
_exptl_crystal_size_min          0.200
_refine_diff_density_max         3.271
_refine_diff_density_min         -2.801
_refine_diff_density_rms         0.463
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.056
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     592
_refine_ls_number_reflns         7059
_refine_ls_number_restraints     702
_refine_ls_restrained_S_all      1.008
_refine_ls_R_factor_all          0.1101
_refine_ls_R_factor_gt           0.1040
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+1294.9978P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2274
_refine_ls_wR_factor_ref         0.2306
_reflns_Friedel_coverage         0.000
_reflns_number_gt                6455
_reflns_number_total             7059
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c5dt04413h2.cif
_cod_data_source_block           shelx_4
_cod_depositor_comments
'Adding full bibliography for 7037670--7037674.cif.'
_cod_database_code               7037673
_shelx_shelxl_version_number     2014/7
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.058
_shelx_estimated_absorpt_t_max   0.112
_exptl_absorpt_special_details
;
 R(int) was 0.0478 before and 0.0456 after correction.
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
W1 W 0.71360(12) -0.16093(11) 0.03740(7) 0.0281(3) Uani 1 1 d . . .
W2 W 0.46148(14) -0.13983(11) -0.13766(8) 0.0346(4) Uani 1 1 d . . .
W4 W 0.49505(15) 0.12069(12) -0.13311(8) 0.0382(4) Uani 1 1 d . . .
W5 W 0.75545(12) -0.01768(10) 0.17519(7) 0.0291(3) Uani 1 1 d . . .
W7 W 0.46246(14) -0.26084(10) -0.00645(8) 0.0366(4) Uani 1 1 d . . .
W8 W 0.74896(12) 0.09949(11) 0.04060(8) 0.0314(4) Uani 1 1 d . . .
Ge1 Ge 0.5000 0.0000 0.0000 0.0245(10) Uani 1 2 d S . P
Cu1 Cu 0.8724(4) 0.2977(4) -0.0226(2) 0.0390(11) Uani 1 1 d . . .
Cu2 Cu 0.9309(4) -0.3878(3) 0.1233(2) 0.0351(10) Uani 1 1 d . . .
Cl1 Cl 0.9521(11) 0.3976(7) -0.0959(6) 0.050(3) Uani 1 1 d . . .
O1 O 0.528(5) -0.113(5) -0.022(3) 0.057(5) Uani 0.5 1 d . U P
O2 O 0.559(5) 0.096(5) -0.018(3) 0.056(5) Uani 0.5 1 d . U P
O3 O 0.641(5) -0.020(5) 0.050(3) 0.055(6) Uani 0.5 1 d . U P
O4 O 0.437(5) 0.001(5) -0.089(3) 0.058(5) Uani 0.5 1 d . U P
O8 O 0.494(3) 0.229(3) -0.0846(18) 0.069(6) Uani 1 1 d . U .
O10 O 0.768(3) -0.126(2) 0.1295(17) 0.057(5) Uani 1 1 d . U .
O11 O 0.322(3) -0.205(3) -0.0480(18) 0.061(5) Uani 1 1 d . U .
O14 O 0.498(3) -0.013(3) -0.1575(19) 0.066(5) Uani 1 1 d . U .
O17 O 0.613(3) -0.169(3) -0.0655(18) 0.064(4) Uani 1 1 d . U .
O18 O 0.432(3) -0.243(3) -0.0962(17) 0.061(5) Uani 1 1 d . U .
O19 O 0.648(3) 0.107(3) -0.0593(18) 0.066(5) Uani 1 1 d . U .
O20 O 0.320(3) -0.092(3) -0.1779(19) 0.064(5) Uani 1 1 d . U .
O21 O 0.862(2) 0.149(2) 0.0569(15) 0.048(6) Uani 1 1 d . U .
O23 O 0.333(3) 0.105(3) -0.1885(19) 0.067(6) Uani 1 1 d . U .
O24 O 0.495(2) 0.177(2) -0.1942(15) 0.044(6) Uani 1 1 d . U .
O25 O 0.877(3) -0.027(2) 0.2564(17) 0.056(7) Uani 1 1 d . U .
O26 O 0.765(3) -0.033(2) 0.0269(16) 0.053(5) Uani 1 1 d . U .
O27 O 0.618(3) -0.253(3) 0.0360(17) 0.062(5) Uani 1 1 d . U .
O29 O 0.438(2) -0.3829(19) -0.0096(15) 0.042(6) Uani 1 1 d . U .
O30 O 0.807(3) 0.545(2) 0.0386(16) 0.060(8) Uani 1 1 d . U .
O31 O 0.867(2) 0.404(2) 0.0274(14) 0.045(6) Uani 1 1 d . U .
O32 O 0.716(2) 0.320(2) -0.1048(16) 0.049(6) Uani 1 1 d . U .
O33 O 0.444(2) -0.207(2) -0.2043(15) 0.048(6) Uani 1 1 d . U .
O34 O 0.818(3) -0.233(2) 0.0558(15) 0.045(6) Uani 1 1 d . U .
O50 O 0.793(3) 0.069(2) 0.1326(17) 0.056(5) Uani 1 1 d . U .
N1 N 1.036(2) 0.282(2) 0.0492(16) 0.030(7) Uani 1 1 d . . .
N2 N 0.884(2) 0.178(2) -0.0647(14) 0.028(6) Uani 1 1 d . . .
N3 N 1.026(2) -0.300(2) 0.2067(15) 0.032(7) Uani 1 1 d . . .
N4 N 0.840(2) -0.391(2) 0.1578(16) 0.032(7) Uani 1 1 d . . .
C1 C 1.109(3) 0.338(4) 0.1032(19) 0.049(12) Uani 1 1 d . . .
H1 H 1.0828 0.3912 0.1136 0.059 Uiso 1 1 calc R U .
C2 C 1.216(4) 0.323(3) 0.143(2) 0.047(10) Uani 1 1 d . . .
H2 H 1.2639 0.3695 0.1772 0.056 Uiso 1 1 calc R U .
C3 C 1.259(3) 0.242(4) 0.136(2) 0.048(11) Uani 1 1 d . . .
H3 H 1.3355 0.2280 0.1682 0.058 Uiso 1 1 calc R U .
C4 C 1.187(3) 0.181(3) 0.078(2) 0.045(10) Uani 1 1 d . U .
H4 H 1.2165 0.1268 0.0701 0.055 Uiso 1 1 calc R U .
C5 C 1.073(3) 0.197(3) 0.031(2) 0.034(8) Uani 1 1 d . U .
C6 C 0.988(3) 0.149(2) -0.0295(17) 0.026(7) Uani 1 1 d . U .
C7 C 1.007(4) 0.061(3) -0.056(2) 0.049(10) Uani 1 1 d . U .
H7 H 1.0781 0.0334 -0.0284 0.059 Uiso 1 1 calc R U .
C8 C 0.928(3) 0.021(3) -0.115(2) 0.045(10) Uani 1 1 d . U .
H8 H 0.9446 -0.0299 -0.1333 0.054 Uiso 1 1 calc R U .
C9 C 0.820(4) 0.054(3) -0.151(2) 0.047(10) Uani 1 1 d . . .
H9 H 0.7602 0.0220 -0.1914 0.056 Uiso 1 1 calc R U .
C10 C 0.802(3) 0.137(3) -0.124(2) 0.037(9) Uani 1 1 d . U .
H10 H 0.7302 0.1631 -0.1493 0.045 Uiso 1 1 calc R U .
C11 C 1.121(4) -0.257(4) 0.231(2) 0.055(12) Uani 1 1 d . . .
H11 H 1.1515 -0.2719 0.2084 0.066 Uiso 1 1 calc R U .
C12 C 1.178(3) -0.194(3) 0.285(2) 0.042(9) Uani 1 1 d . U .
H12 H 1.2421 -0.1630 0.2962 0.050 Uiso 1 1 calc R U .
C13 C 1.141(4) -0.175(3) 0.321(2) 0.051(11) Uani 1 1 d . U .
H13 H 1.1841 -0.1358 0.3613 0.061 Uiso 1 1 calc R U .
C14 C 1.044(4) -0.213(3) 0.302(2) 0.046(10) Uani 1 1 d . U .
H14 H 1.0168 -0.1943 0.3257 0.055 Uiso 1 1 calc R U .
C15 C 0.980(3) -0.283(3) 0.2414(19) 0.033(8) Uani 1 1 d . U .
C16 C 0.881(3) -0.330(3) 0.217(2) 0.038(9) Uani 1 1 d . U .
C17 C 0.818(5) -0.316(4) 0.241(3) 0.069(16) Uani 1 1 d . . .
H17 H 0.8429 -0.2750 0.2790 0.083 Uiso 1 1 calc R U .
C18 C 0.718(4) -0.366(4) 0.206(3) 0.063(14) Uani 1 1 d . . .
H18 H 0.6746 -0.3572 0.2207 0.076 Uiso 1 1 calc R U .
C19 C 0.680(4) -0.425(3) 0.153(2) 0.047(10) Uani 1 1 d . U .
H19 H 0.6133 -0.4598 0.1313 0.057 Uiso 1 1 calc R U .
C20 C 0.745(3) -0.436(3) 0.128(2) 0.038(9) Uani 1 1 d . . .
H20 H 0.7172 -0.4760 0.0890 0.046 Uiso 1 1 calc R U .
C22 C 0.622(3) 0.553(3) -0.099(2) 0.041(9) Uani 1 1 d . U .
H22 H 0.6397 0.6074 -0.0696 0.049 Uiso 1 1 calc R U .
C23 C 0.526(4) 0.559(3) -0.167(3) 0.057(13) Uani 1 1 d . . .
H23 H 0.4791 0.6132 -0.1821 0.069 Uiso 1 1 calc R U .
C24 C 0.500(3) 0.482(3) -0.214(2) 0.043(9) Uani 1 1 d . U .
N5 N 0.569(3) 0.400(2) -0.1871(17) 0.038(7) Uani 1 1 d . U .
C26 C 0.668(3) 0.393(3) -0.1175(19) 0.031(8) Uani 1 1 d . U .
C27 C 0.692(3) 0.474(3) -0.0700(19) 0.030(8) Uani 1 1 d . . .
C28 C 0.794(3) 0.476(3) 0.003(2) 0.031(8) Uani 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O34 W1 O10 100.1(14) . .
O34 W1 O27 102.2(15) . .
O10 W1 O27 87.8(14) . .
O34 W1 O17 100.1(14) . .
O10 W1 O17 159.7(15) . .
O27 W1 O17 87.1(14) . .
O34 W1 O26 99.3(14) . .
O10 W1 O26 90.6(13) . .
O27 W1 O26 158.3(14) . .
O17 W1 O26 87.0(13) . .
O34 W1 O3 153.6(19) . .
O10 W1 O3 62.5(19) . .
O27 W1 O3 97.0(19) . .
O17 W1 O3 98.8(19) . .
O26 W1 O3 63.4(18) . .
O34 W1 O1 156.2(19) . .
O10 W1 O1 98.2(19) . .
O27 W1 O1 63.5(19) . .
O17 W1 O1 62.1(19) . .
O26 W1 O1 95.5(19) . .
O3 W1 O1 50(2) . .
O33 W2 O20 103.8(15) . .
O33 W2 O17 98.4(15) . .
O20 W2 O17 157.5(16) . .
O33 W2 O18 98.6(15) . .
O20 W2 O18 87.8(15) . .
O17 W2 O18 85.1(14) . .
O33 W2 O14 98.0(15) . .
O20 W2 O14 88.6(15) . .
O17 W2 O14 92.2(14) . .
O18 W2 O14 163.4(15) . .
O33 W2 O1 154.6(19) . .
O20 W2 O1 94.6(19) . .
O17 W2 O1 63.1(19) . .
O18 W2 O1 64.2(19) . .
O14 W2 O1 99.9(19) . .
O33 W2 O4 154.3(19) . .
O20 W2 O4 59.4(19) . .
O17 W2 O4 100.8(19) . .
O18 W2 O4 99.9(19) . .
O14 W2 O4 64.5(19) . .
O1 W2 O4 51(2) . .
O24 W4 O19 102.3(15) . .
O24 W4 O8 101.1(16) . .
O19 W4 O8 88.1(14) . .
O24 W4 O14 98.8(15) . .
O19 W4 O14 87.1(14) . .
O8 W4 O14 160.1(16) . .
O24 W4 O23 97.3(15) . .
O19 W4 O23 160.2(16) . .
O8 W4 O23 90.9(15) . .
O14 W4 O23 87.1(15) . .
O24 W4 O2 153.4(19) . .
O19 W4 O2 59.3(19) . .
O8 W4 O2 62(2) . .
O14 W4 O2 99(2) . .
O23 W4 O2 103.0(19) . .
O24 W4 O4 155.4(19) . .
O19 W4 O4 95(2) . .
O8 W4 O4 96(2) . .
O14 W4 O4 64.9(19) . .
O23 W4 O4 65.0(19) . .
O2 W4 O4 51(2) . .
O25 W5 O50 101.6(15) . .
O25 W5 O20 106.0(15) . 3_655
O50 W5 O20 85.7(15) . 3_655
O25 W5 O10 100.5(15) . .
O50 W5 O10 89.8(13) . .
O20 W5 O10 153.5(15) 3_655 .
O25 W5 O23 97.7(15) . 3_655
O50 W5 O23 160.7(15) . 3_655
O20 W5 O23 88.6(14) 3_655 3_655
O10 W5 O23 87.2(14) . 3_655
O25 W5 O4 157(2) . 3_655
O50 W5 O4 95.3(19) . 3_655
O20 W5 O4 59.8(19) 3_655 3_655
O10 W5 O4 94.8(19) . 3_655
O23 W5 O4 65.9(19) 3_655 3_655
O25 W5 O3 154.2(19) . .
O50 W5 O3 63.0(18) . .
O20 W5 O3 93.9(19) 3_655 .
O10 W5 O3 61.1(18) . .
O23 W5 O3 99.1(19) 3_655 .
O4 W5 O3 49(2) 3_655 .
O29 W7 O11 102.9(14) . .
O29 W7 O8 100.6(15) . 3_655
O11 W7 O8 89.9(14) . 3_655
O29 W7 O27 104.1(14) . .
O11 W7 O27 153.0(15) . .
O8 W7 O27 86.2(15) 3_655 .
O29 W7 O18 100.3(14) . .
O11 W7 O18 86.7(14) . .
O8 W7 O18 159.0(16) 3_655 .
O27 W7 O18 87.5(14) . .
O29 W7 O1 157.6(19) . .
O11 W7 O1 91.5(19) . .
O8 W7 O1 96(2) 3_655 .
O27 W7 O1 62.4(18) . .
O18 W7 O1 63.1(19) . .
O29 W7 O2 150.2(18) . 3_655
O11 W7 O2 57.9(18) . 3_655
O8 W7 O2 60.3(19) 3_655 3_655
O27 W7 O2 97.5(19) . 3_655
O18 W7 O2 100.9(19) . 3_655
O1 W7 O2 52(2) . 3_655
O21 W8 O26 101.8(14) . .
O21 W8 O11 104.2(15) . 3_655
O26 W8 O11 154.0(14) . 3_655
O21 W8 O19 101.0(15) . .
O26 W8 O19 85.6(14) . .
O11 W8 O19 90.7(14) 3_655 .
O21 W8 O50 103.9(14) . .
O26 W8 O50 90.3(13) . .
O11 W8 O50 82.3(14) 3_655 .
O19 W8 O50 155.1(15) . .
O21 W8 O2 152(2) . .
O26 W8 O2 96.9(19) . .
O11 W8 O2 59.6(19) 3_655 .
O19 W8 O2 59.3(19) . .
O50 W8 O2 97.0(19) . .
O21 W8 O3 156.6(19) . .
O26 W8 O3 62.6(17) . .
O11 W8 O3 92.2(18) 3_655 .
O19 W8 O3 95.3(19) . .
O50 W8 O3 61.3(18) . .
O2 W8 O3 52(2) . .
O3 Ge1 O3 180.0 3_655 .
O3 Ge1 O4 112(3) 3_655 3_655
O3 Ge1 O4 68(3) . 3_655
O3 Ge1 O4 68(3) 3_655 .
O3 Ge1 O4 112(3) . .
O4 Ge1 O4 180.0 3_655 .
O3 Ge1 O1 111(3) 3_655 .
O3 Ge1 O1 69(3) . .
O4 Ge1 O1 109(3) 3_655 .
O4 Ge1 O1 71(3) . .
O3 Ge1 O1 69(3) 3_655 3_655
O3 Ge1 O1 111(3) . 3_655
O4 Ge1 O1 71(3) 3_655 3_655
O4 Ge1 O1 109(3) . 3_655
O1 Ge1 O1 180.0 . 3_655
O3 Ge1 O2 108(3) 3_655 .
O3 Ge1 O2 72(3) . .
O4 Ge1 O2 110(3) 3_655 .
O4 Ge1 O2 70(3) . .
O1 Ge1 O2 108(3) . .
O1 Ge1 O2 72(3) 3_655 .
O3 Ge1 O2 72(3) 3_655 3_655
O3 Ge1 O2 108(3) . 3_655
O4 Ge1 O2 70(3) 3_655 3_655
O4 Ge1 O2 110(3) . 3_655
O1 Ge1 O2 72(3) . 3_655
O1 Ge1 O2 108(3) 3_655 3_655
O2 Ge1 O2 180.0 . 3_655
O31 Cu1 O32 91.2(12) . .
O31 Cu1 N2 173.1(12) . .
O32 Cu1 N2 92.6(12) . .
O31 Cu1 N1 93.0(12) . .
O32 Cu1 N1 170.1(13) . .
N2 Cu1 N1 84.2(12) . .
O30 Cu2 N3 165.4(13) 1_545 .
O30 Cu2 N4 87.6(14) 1_545 .
N3 Cu2 N4 81.2(13) . .
O30 Cu2 Cl1 95.4(11) 1_545 3_755
N3 Cu2 Cl1 96.9(10) . 3_755
N4 Cu2 Cl1 172.7(9) . 3_755
Ge1 O1 W2 120(3) . .
Ge1 O1 W1 119(3) . .
W2 O1 W1 99(2) . .
Ge1 O1 W7 119(3) . .
W2 O1 W7 98(2) . .
W1 O1 W7 98(2) . .
Ge1 O2 W8 119(3) . .
Ge1 O2 W4 120(3) . .
W8 O2 W4 100(2) . .
Ge1 O2 W7 117(3) . 3_655
W8 O2 W7 98(2) . 3_655
W4 O2 W7 98(2) . 3_655
Ge1 O3 W1 122(3) . .
Ge1 O3 W5 121(3) . .
W1 O3 W5 98(2) . .
Ge1 O3 W8 117(3) . .
W1 O3 W8 98(2) . .
W5 O3 W8 96(2) . .
Ge1 O4 W5 122(3) . 3_655
Ge1 O4 W2 118(3) . .
W5 O4 W2 98(2) 3_655 .
Ge1 O4 W4 119(3) . .
W5 O4 W4 98(2) 3_655 .
W2 O4 W4 97(2) . .
W4 O8 W7 139(2) . 3_655
W1 O10 W5 137.6(18) . .
W7 O11 W8 143(2) . 3_655
W4 O14 W2 134(2) . .
W2 O17 W1 135(2) . .
W7 O18 W2 134.5(19) . .
W4 O19 W8 141(2) . .
W2 O20 W5 142(2) . 3_655
W4 O23 W5 130.7(19) . 3_655
W8 O26 W1 135.9(16) . .
W1 O27 W7 136.4(19) . .
C28 O30 Cu2 138(3) . 1_565
C28 O31 Cu1 129(2) . .
C26 O32 Cu1 125(3) . .
W5 O50 W8 139.5(18) . .
C1 N1 C5 121(3) . .
C1 N1 Cu1 130(3) . .
C5 N1 Cu1 109(2) . .
C10 N2 C6 122(3) . .
C10 N2 Cu1 126(3) . .
C6 N2 Cu1 112(2) . .
C11 N3 C15 118(3) . .
C11 N3 Cu2 129(3) . .
C15 N3 Cu2 113(2) . .
C20 N4 C16 118(3) . .
C20 N4 Cu2 127(3) . .
C16 N4 Cu2 115(2) . .
C2 C1 N1 123(4) . .
C2 C1 H1 118.4 . .
N1 C1 H1 118.4 . .
C1 C2 C3 122(5) . .
C1 C2 H2 119.1 . .
C3 C2 H2 119.1 . .
C2 C3 C4 118(4) . .
C2 C3 H3 121.2 . .
C4 C3 H3 121.2 . .
C5 C4 C3 123(4) . .
C5 C4 H4 118.7 . .
C3 C4 H4 118.7 . .
C6 C5 C4 133(4) . .
C6 C5 N1 114(3) . .
C4 C5 N1 113(3) . .
N2 C6 C5 121(3) . .
N2 C6 C7 117(3) . .
C5 C6 C7 122(3) . .
C8 C7 C6 122(4) . .
C8 C7 H7 119.0 . .
C6 C7 H7 119.0 . .
C7 C8 C9 119(4) . .
C7 C8 H8 120.3 . .
C9 C8 H8 120.3 . .
C8 C9 C10 118(4) . .
C8 C9 H9 121.2 . .
C10 C9 H9 121.2 . .
N2 C10 C9 122(4) . .
N2 C10 H10 119.2 . .
C9 C10 H10 119.2 . .
N3 C11 C12 127(4) . .
N3 C11 H11 116.6 . .
C12 C11 H11 116.6 . .
C13 C12 C11 119(4) . .
C13 C12 H12 120.7 . .
C11 C12 H12 120.7 . .
C12 C13 C14 121(5) . .
C12 C13 H13 119.4 . .
C14 C13 H13 119.4 . .
C13 C14 C15 120(4) . .
C13 C14 H14 119.9 . .
C15 C14 H14 119.9 . .
C16 C15 N3 119(3) . .
C16 C15 C14 127(4) . .
N3 C15 C14 115(3) . .
C15 C16 C17 127(4) . .
C15 C16 N4 112(3) . .
C17 C16 N4 121(4) . .
C18 C17 C16 117(5) . .
C18 C17 H17 121.4 . .
C16 C17 H17 121.4 . .
C19 C18 C17 124(5) . .
C19 C18 H18 118.1 . .
C17 C18 H18 118.1 . .
C18 C19 C20 118(4) . .
C18 C19 H19 121.1 . .
C20 C19 H19 121.1 . .
N4 C20 C19 123(4) . .
N4 C20 H20 118.6 . .
C19 C20 H20 118.6 . .
C27 C22 C23 125(4) . .
C27 C22 H22 117.5 . .
C23 C22 H22 117.5 . .
C22 C23 C24 119(4) . .
C22 C23 H23 120.3 . .
C24 C23 H23 120.3 . .
N5 C24 C23 118(4) . .
C24 N5 C26 124(3) . .
O32 C26 N5 114(3) . .
O32 C26 C27 129(4) . .
N5 C26 C27 117(3) . .
C22 C27 C28 121(3) . .
C22 C27 C26 117(3) . .
C28 C27 C26 121(3) . .
O30 C28 O31 122(3) . .
O30 C28 C27 117(3) . .
O31 C28 C27 121(3) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
W1 O34 1.67(3) .
W1 O10 1.88(3) .
W1 O27 1.90(3) .
W1 O17 1.94(3) .
W1 O26 1.97(3) .
W1 O3 2.31(6) .
W1 O1 2.32(6) .
W2 O33 1.71(3) .
W2 O20 1.84(3) .
W2 O17 1.88(3) .
W2 O18 1.92(3) .
W2 O14 1.95(4) .
W2 O1 2.31(6) .
W2 O4 2.37(7) .
W4 O24 1.65(3) .
W4 O19 1.86(3) .
W4 O8 1.88(3) .
W4 O14 1.91(4) .
W4 O23 1.95(3) .
W4 O2 2.31(6) .
W4 O4 2.37(7) .
W5 O25 1.66(3) .
W5 O50 1.86(3) .
W5 O20 1.90(3) 3_655
W5 O10 1.91(3) .
W5 O23 1.96(4) 3_655
W5 O4 2.32(6) 3_655
W5 O3 2.36(6) .
W7 O29 1.68(3) .
W7 O11 1.86(3) .
W7 O8 1.90(3) 3_655
W7 O27 1.90(3) .
W7 O18 1.92(3) .
W7 O1 2.37(7) .
W7 O2 2.37(6) 3_655
W8 O21 1.65(3) .
W8 O26 1.86(3) .
W8 O11 1.86(3) 3_655
W8 O19 1.89(3) .
W8 O50 1.91(3) .
W8 O2 2.29(6) .
W8 O3 2.41(6) .
Ge1 O3 1.71(6) 3_655
Ge1 O3 1.71(6) .
Ge1 O4 1.73(6) 3_655
Ge1 O4 1.73(6) .
Ge1 O1 1.75(7) .
Ge1 O1 1.75(7) 3_655
Ge1 O2 1.78(7) .
Ge1 O2 1.78(7) 3_655
Cu1 O31 1.90(3) .
Cu1 O32 1.96(3) .
Cu1 N2 1.97(3) .
Cu1 N1 1.98(3) .
Cu2 O30 1.94(3) 1_545
Cu2 N3 1.98(3) .
Cu2 N4 1.99(3) .
Cu2 Cl1 2.240(12) 3_755
Cl1 Cu2 2.240(12) 3_755
O2 W7 2.37(6) 3_655
O4 W5 2.32(6) 3_655
O8 W7 1.90(3) 3_655
O11 W8 1.86(3) 3_655
O20 W5 1.90(3) 3_655
O23 W5 1.96(4) 3_655
O30 C28 1.20(4) .
O30 Cu2 1.94(3) 1_565
O31 C28 1.31(4) .
O32 C26 1.15(4) .
N1 C1 1.30(5) .
N1 C5 1.46(5) .
N2 C10 1.30(5) .
N2 C6 1.31(4) .
N3 C11 1.31(6) .
N3 C15 1.39(5) .
N4 C20 1.31(5) .
N4 C16 1.41(5) .
C1 C2 1.29(6) .
C1 H1 0.9300 .
C2 C3 1.33(6) .
C2 H2 0.9300 .
C3 C4 1.40(6) .
C3 H3 0.9300 .
C4 C5 1.37(5) .
C4 H4 0.9300 .
C5 C6 1.37(5) .
C6 C7 1.45(5) .
C7 C8 1.28(6) .
C7 H7 0.9300 .
C8 C9 1.38(6) .
C8 H8 0.9300 .
C9 C10 1.39(5) .
C9 H9 0.9300 .
C10 H10 0.9300 .
C11 C12 1.33(6) .
C11 H11 0.9300 .
C12 C13 1.31(6) .
C12 H12 0.9300 .
C13 C14 1.34(6) .
C13 H13 0.9300 .
C14 C15 1.48(6) .
C14 H14 0.9300 .
C15 C16 1.38(5) .
C16 C17 1.39(6) .
C17 C18 1.37(7) .
C17 H17 0.9300 .
C18 C19 1.30(7) .
C18 H18 0.9300 .
C19 C20 1.42(6) .
C19 H19 0.9300 .
C20 H20 0.9300 .
C22 C27 1.36(5) .
C22 C23 1.36(6) .
C22 H22 0.9300 .
C23 C24 1.39(7) .
C23 H23 0.9300 .
C24 N5 1.38(5) .
N5 C26 1.40(5) .
C26 C27 1.46(5) .
C27 C28 1.45(5) .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O3 Ge1 O1 W2 58(4) 3_655 .
O3 Ge1 O1 W2 -122(4) . .
O4 Ge1 O1 W2 -179(3) 3_655 .
O4 Ge1 O1 W2 1(3) . .
O2 Ge1 O1 W2 -60(4) . .
O2 Ge1 O1 W2 120(4) 3_655 .
O3 Ge1 O1 W1 180(3) 3_655 .
O3 Ge1 O1 W1 0(3) . .
O4 Ge1 O1 W1 -57(4) 3_655 .
O4 Ge1 O1 W1 123(4) . .
O2 Ge1 O1 W1 62(4) . .
O2 Ge1 O1 W1 -118(4) 3_655 .
O3 Ge1 O1 W7 -62(4) 3_655 .
O3 Ge1 O1 W7 118(4) . .
O4 Ge1 O1 W7 62(4) 3_655 .
O4 Ge1 O1 W7 -118(4) . .
O2 Ge1 O1 W7 -180(3) . .
O2 Ge1 O1 W7 0(3) 3_655 .
O3 Ge1 O2 W8 179(3) 3_655 .
O3 Ge1 O2 W8 -1(3) . .
O4 Ge1 O2 W8 57(4) 3_655 .
O4 Ge1 O2 W8 -123(4) . .
O1 Ge1 O2 W8 -62(4) . .
O1 Ge1 O2 W8 118(4) 3_655 .
O3 Ge1 O2 W4 -58(4) 3_655 .
O3 Ge1 O2 W4 122(4) . .
O4 Ge1 O2 W4 -180(3) 3_655 .
O4 Ge1 O2 W4 0(3) . .
O1 Ge1 O2 W4 62(4) . .
O1 Ge1 O2 W4 -118(4) 3_655 .
O3 Ge1 O2 W7 61(4) 3_655 3_655
O3 Ge1 O2 W7 -119(4) . 3_655
O4 Ge1 O2 W7 -61(4) 3_655 3_655
O4 Ge1 O2 W7 119(4) . 3_655
O1 Ge1 O2 W7 -180(3) . 3_655
O1 Ge1 O2 W7 0(3) 3_655 3_655
O4 Ge1 O3 W1 122(4) 3_655 .
O4 Ge1 O3 W1 -58(4) . .
O1 Ge1 O3 W1 0(3) . .
O1 Ge1 O3 W1 -180(3) 3_655 .
O2 Ge1 O3 W1 -118(4) . .
O2 Ge1 O3 W1 62(4) 3_655 .
O4 Ge1 O3 W5 -3(3) 3_655 .
O4 Ge1 O3 W5 177(3) . .
O1 Ge1 O3 W5 -125(4) . .
O1 Ge1 O3 W5 55(4) 3_655 .
O2 Ge1 O3 W5 117(4) . .
O2 Ge1 O3 W5 -63(4) 3_655 .
O4 Ge1 O3 W8 -119(4) 3_655 .
O4 Ge1 O3 W8 61(4) . .
O1 Ge1 O3 W8 119(4) . .
O1 Ge1 O3 W8 -61(4) 3_655 .
O2 Ge1 O3 W8 1(3) . .
O2 Ge1 O3 W8 -179(3) 3_655 .
O3 Ge1 O4 W5 -3(3) 3_655 3_655
O3 Ge1 O4 W5 177(3) . 3_655
O1 Ge1 O4 W5 120(4) . 3_655
O1 Ge1 O4 W5 -60(4) 3_655 3_655
O2 Ge1 O4 W5 -123(4) . 3_655
O2 Ge1 O4 W5 57(4) 3_655 3_655
O3 Ge1 O4 W2 -124(4) 3_655 .
O3 Ge1 O4 W2 56(4) . .
O1 Ge1 O4 W2 -1(3) . .
O1 Ge1 O4 W2 179(3) 3_655 .
O2 Ge1 O4 W2 116(4) . .
O2 Ge1 O4 W2 -64(4) 3_655 .
O3 Ge1 O4 W4 119(4) 3_655 .
O3 Ge1 O4 W4 -61(4) . .
O1 Ge1 O4 W4 -118(4) . .
O1 Ge1 O4 W4 62(4) 3_655 .
O2 Ge1 O4 W4 0(3) . .
O2 Ge1 O4 W4 180(3) 3_655 .
O24 W4 O8 W7 -155(3) . 3_655
O19 W4 O8 W7 -53(3) . 3_655
O14 W4 O8 W7 23(7) . 3_655
O23 W4 O8 W7 108(3) . 3_655
O2 W4 O8 W7 3(3) . 3_655
O4 W4 O8 W7 43(4) . 3_655
O34 W1 O10 W5 151(3) . .
O27 W1 O10 W5 -107(3) . .
O17 W1 O10 W5 -31(6) . .
O26 W1 O10 W5 51(3) . .
O3 W1 O10 W5 -8(3) . .
O1 W1 O10 W5 -44(3) . .
O29 W7 O11 W8 140(3) . 3_655
O8 W7 O11 W8 39(3) 3_655 3_655
O27 W7 O11 W8 -42(5) . 3_655
O18 W7 O11 W8 -120(3) . 3_655
O1 W7 O11 W8 -57(4) . 3_655
O2 W7 O11 W8 -15(3) 3_655 3_655
O33 W2 O17 W1 -162(3) . .
O20 W2 O17 W1 8(6) . .
O18 W2 O17 W1 -64(3) . .
O14 W2 O17 W1 100(3) . .
O1 W2 O17 W1 0(3) . .
O4 W2 O17 W1 35(3) . .
O24 W4 O19 W8 151(3) . .
O8 W4 O19 W8 50(3) . .
O14 W4 O19 W8 -110(3) . .
O23 W4 O19 W8 -37(6) . .
O2 W4 O19 W8 -8(3) . .
O4 W4 O19 W8 -46(3) . .
O21 W8 O19 W4 -150(3) . .
O26 W8 O19 W4 109(3) . .
O11 W8 O19 W4 -46(3) 3_655 .
O50 W8 O19 W4 27(6) . .
O2 W8 O19 W4 8(3) . .
O3 W8 O19 W4 47(3) . .
O33 W2 O20 W5 -149(3) . 3_655
O17 W2 O20 W5 41(6) . 3_655
O18 W2 O20 W5 113(3) . 3_655
O14 W2 O20 W5 -51(3) . 3_655
O1 W2 O20 W5 49(4) . 3_655
O4 W2 O20 W5 10(3) . 3_655
O21 W8 O26 W1 154(2) . .
O11 W8 O26 W1 -24(5) 3_655 .
O19 W8 O26 W1 -106(3) . .
O50 W8 O26 W1 49(3) . .
O2 W8 O26 W1 -48(3) . .
O3 W8 O26 W1 -8(3) . .
O34 W1 O27 W7 -156(3) . .
O10 W1 O27 W7 104(3) . .
O17 W1 O27 W7 -56(3) . .
O26 W1 O27 W7 19(6) . .
O3 W1 O27 W7 43(3) . .
O1 W1 O27 W7 4(3) . .
O25 W5 O50 W8 152(3) . .
O20 W5 O50 W8 -103(3) 3_655 .
O10 W5 O50 W8 51(3) . .
O23 W5 O50 W8 -30(6) 3_655 .
O4 W5 O50 W8 -44(3) 3_655 .
O3 W5 O50 W8 -6(3) . .
C5 N1 C1 C2 1(6) . .
Cu1 N1 C1 C2 -174(3) . .
N1 C1 C2 C3 -7(7) . .
C1 C2 C3 C4 8(7) . .
C2 C3 C4 C5 -4(7) . .
C3 C4 C5 C6 178(4) . .
C3 C4 C5 N1 -1(6) . .
C1 N1 C5 C6 -176(4) . .
Cu1 N1 C5 C6 0(4) . .
C1 N1 C5 C4 3(5) . .
Cu1 N1 C5 C4 179(3) . .
C10 N2 C6 C5 177(3) . .
Cu1 N2 C6 C5 3(4) . .
C10 N2 C6 C7 -7(5) . .
Cu1 N2 C6 C7 -180(3) . .
C4 C5 C6 N2 179(4) . .
N1 C5 C6 N2 -2(5) . .
C4 C5 C6 C7 2(7) . .
N1 C5 C6 C7 -179(3) . .
N2 C6 C7 C8 8(6) . .
C5 C6 C7 C8 -175(4) . .
C6 C7 C8 C9 -8(7) . .
C7 C8 C9 C10 6(7) . .
C6 N2 C10 C9 5(6) . .
Cu1 N2 C10 C9 177(3) . .
C8 C9 C10 N2 -5(6) . .
C15 N3 C11 C12 -3(6) . .
Cu2 N3 C11 C12 175(3) . .
N3 C11 C12 C13 4(7) . .
C11 C12 C13 C14 -6(7) . .
C12 C13 C14 C15 5(7) . .
C11 N3 C15 C16 -179(4) . .
Cu2 N3 C15 C16 3(4) . .
C11 N3 C15 C14 2(5) . .
Cu2 N3 C15 C14 -176(3) . .
C13 C14 C15 C16 178(4) . .
C13 C14 C15 N3 -4(6) . .
N3 C15 C16 C17 -175(4) . .
C14 C15 C16 C17 4(7) . .
N3 C15 C16 N4 0(5) . .
C14 C15 C16 N4 179(4) . .
C20 N4 C16 C15 -177(3) . .
Cu2 N4 C16 C15 -3(4) . .
C20 N4 C16 C17 -2(5) . .
Cu2 N4 C16 C17 172(3) . .
C15 C16 C17 C18 176(4) . .
N4 C16 C17 C18 2(6) . .
C16 C17 C18 C19 1(7) . .
C17 C18 C19 C20 -3(7) . .
C16 N4 C20 C19 0(6) . .
Cu2 N4 C20 C19 -173(3) . .
C18 C19 C20 N4 2(7) . .
C27 C22 C23 C24 -5(7) . .
C22 C23 C24 N5 4(6) . .
C23 C24 N5 C26 -4(6) . .
Cu1 O32 C26 N5 163(2) . .
Cu1 O32 C26 C27 -21(6) . .
C24 N5 C26 O32 -179(4) . .
C24 N5 C26 C27 4(5) . .
C23 C22 C27 C28 178(4) . .
C23 C22 C27 C26 4(6) . .
O32 C26 C27 C22 180(4) . .
N5 C26 C27 C22 -4(5) . .
O32 C26 C27 C28 6(6) . .
N5 C26 C27 C28 -178(3) . .
Cu2 O30 C28 O31 24(7) 1_565 .
Cu2 O30 C28 C27 -157(3) 1_565 .
Cu1 O31 C28 O30 -171(3) . .
Cu1 O31 C28 C27 10(5) . .
C22 C27 C28 O30 8(6) . .
C26 C27 C28 O30 -179(4) . .
C22 C27 C28 O31 -173(4) . .
C26 C27 C28 O31 1(5) . .
